Influencing the Morphology and Phase of Calcium Ceramic Nanoparticles Based on the Calcium Alkoxide Precursors' Characteristics
Boyle, Timothy J.; Hernandez-Sanchez, Bernadette A.; Baros, Christina M.; Brewer, Luke N.; Rodriguez, Mark A.; Chemistry of Materials 19 (2007) 2016–; doi:10.1021/cm0700091

data_4001347
_publ_section_title
;
 Influencing the Morphology and Phase of Calcium Ceramic Nanoparticles
 Based on the Calcium Alkoxide Precursors' Characteristics
;
_journal_issue                   8
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2016
_journal_paper_doi               10.1021/cm0700091
_journal_volume                  19
_journal_year                    2007
_chemical_formula_moiety         'C40 H66 Ca O6, 2(C36 H58 Ca O5), (C4 H8 O)'
_chemical_formula_sum            'C116 H190 Ca3 O17'
_chemical_formula_weight         1972.89
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 111.120(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   40.750(9)
_cell_length_b                   16.333(4)
_cell_length_c                   19.166(4)
_cell_measurement_reflns_used    10973
_cell_measurement_temperature    203(2)
_cell_measurement_theta_max      25.41
_cell_measurement_theta_min      0.919
_cell_volume                     11899(5)
_computing_cell_refinement       'SMART 5.054 (Bruker, 1998)'
_computing_data_collection       'SMART 5.054 (Bruker, 1998)'
_computing_data_reduction        'SAINT 6.02 (Bruker, 2001)'
_computing_molecular_graphics    'SHELXTL 5.1  (Bruker, 1998)'
_computing_publication_material  'SHELXTL 5.1  (Bruker, 1998)'
_computing_structure_refinement  'XSHELL 4.01 (Bruker, 2000)'
_computing_structure_solution    'SHELXTL 5.1  (Bruker, 1998)'
_diffrn_ambient_temperature      203(2)
_diffrn_measured_fraction_theta_full 0.83
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX CCD'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0800
_diffrn_reflns_av_sigmaI/netI    0.0834
_diffrn_reflns_limit_h_max       48
_diffrn_reflns_limit_h_min       -49
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            42621
_diffrn_reflns_theta_full        25.41
_diffrn_reflns_theta_max         25.41
_diffrn_reflns_theta_min         1.36
_diffrn_standards_decay_%        0.973
_diffrn_standards_interval_time  .919
_diffrn_standards_number         604
_exptl_absorpt_coefficient_mu    0.197
_exptl_absorpt_correction_T_max  0.98
_exptl_absorpt_correction_T_min  0.97
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SADABS ver 2.03, Sheldrick (1999).'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.101
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prismatic
_exptl_crystal_F_000             4312
_exptl_crystal_size_max          0.43
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.366
_refine_diff_density_min         -0.278
_refine_diff_density_rms         0.054
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.973
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     604
_refine_ls_number_reflns         10932
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.973
_refine_ls_R_factor_all          0.1312
_refine_ls_R_factor_gt           0.0686
_refine_ls_shift/su_max          0.007
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0875P)^2^+9.4251P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1593
_refine_ls_wR_factor_ref         0.1836
_reflns_number_gt                5799
_reflns_number_total             10932
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm0700091si20070102_085813.cif
_cod_data_source_block           jun291p
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 

The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not_measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_cell_volume        11900(5)
_cod_original_sg_symbol_H-M      'C2/c  '
_cod_database_code               4001347